\documentclass[%
reprint,
superscriptaddress,
%preprint,
nofootinbib,
nobibnotes,
 amsmath,amssymb,
 aps,
%pra,
%prb,
prl,
%rmp,
%floatfix,
11pt,
]{revtex4-1}

\usepackage{graphicx}% Include figure files
\usepackage{dcolumn}% Align table columns on decimal point
\usepackage{bm}% bold math

\usepackage[utf8]{inputenc}
\usepackage[T1]{fontenc}

\usepackage{iftex}
\ifPDFTeX
   \usepackage[utf8]{inputenc}
   \usepackage[T1]{fontenc}
   \usepackage{lmodern}
\else
   \ifXeTeX
     \usepackage{xltxtra}
   \else
     \usepackage{luatextra}
   \fi
   %\setmainfont[Ligatures=TeX]{Linux Libertine O}
   %\setmainfont[Ligatures=TeX]{Arial Unicode MS}
   \setmainfont{FreeSerif}
   \setmonofont{FreeMono}
   \usepackage{polyglossia}
\fi

\usepackage[paperwidth=170mm, paperheight=140mm, margin=20mm]{geometry}
%\usepackage{etoolbox}
\linespread{1.1}%line spacing
\usepackage{setspace}
%\usepackage{caption}
\usepackage{float}

\makeatletter
\def\frontmatter@abstractwidth{370\p@}
%\def\frontmatter@title@above{\addvspace{1pt}}
\def\frontmatter@title@below{} %\addvspace{-10pt}}
%\def\frontmatter@above@affilgroup{\addvspace{-11pt}}
\def\frontmatter@preabstractspace{6\p@}
\def\frontmatter@postabstractspace{3.5\p@}
\def\frontmatter@authorformat{\centering\normalsize\addvspace{1.5\p@}}%
%%\def\frontmatter@authorformat{\centering\advance\baselineskip\p@\parskip0.1\p@\let\thanks\thanks@latex\let\and\and@space}%
%\def\frontmatter@authorbelow{\vskip -12pt}%
\def\frontmatter@abstractfont{\small\parindent0em\relax\adjust@abstractwidth}%
\makeatother

\begin{document}
\title{Temperature dependent magnetic and structural properties of Ni-Mn-Ga Heusler alloy glass-coated microwires}
\author{\underline{S. Shevyrtalov}}
\affiliation{Immanuel Kant Baltic Federal University, Kaliningrad, Russia}
\author{V. Rodionova}
\affiliation{Immanuel Kant Baltic Federal University, Kaliningrad, Russia}
\author{K. Chichay}
\affiliation{Immanuel Kant Baltic Federal University, Kaliningrad, Russia}
\author{V. Zhukova}
\affiliation{Dpto. Fisica de Materiales, Fac. Quimicas, sUPV/EHU, 20009 San Sebastian, Spain}
\author{A. Zhukov}
\affiliation{Dpto. Fisica de Materiales, Fac. Quimicas, sUPV/EHU, 20009 San Sebastian, Spain}
\begin{abstract}
In last years, Ni-Mn-X Heusler alloys have attracted significant attention because of number of their functional properties. Ni-Mn-Ga glass-coated microwires (MWs) have a good prospects for new generation technical applications [1]. 
We investigated magnetic and structural properties of the Ni-Mn-Ga MWs fabricated by Tailor-Ulitovsky method. MWs with total diameter of 54.6 and 24.7 $\mu$m and the diameter of metallic core of 26.7 and 8.3 $\mu$m, respectively, were obtained. Energy dispersive spectrometer (Oxford Instr. X-Act) was used to detect composition of the metallic core of as-cast and annealed MWs. Magnetic moment versus temperature (-196-77$^\circ$ C) measurements and hysteresis loops were obtained by VSM (Lakeshore 7400 system). X-Ray diffraction (using Bruker D8 Discover in temperature range of -100-350 $^\circ$ C) and magnetic temperature measurements reveal martensitic transition in the samples near the room temperature.


\textbf{References:}
\begin{spacing}{0.8}

{\scriptsize[1] A. Zhukov, Journal of Alloys and Compounds 575, 73-79 (2013)}
\end{spacing}

\end{abstract}
\maketitle

\end{document}
